Ternary fluorides Ba<i>M</i>F~4~ (<i>M</i> = Zn, Mg and Mn) at low temperatures
Posse, Jose Maria; Grzechnik, Andrzej; Friese, Karen; Acta Crystallographica Section B 65 (2009) 576–586; doi:10.1107/S0108768109027177

data_2104460
_publ_section_title
;
 Ternary fluorides Ba<i>M</i>F~4~ (<i>M</i> = Zn, Mg and Mn) at low
 temperatures
;
_journal_coeditor_code           SN5085
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              576
_journal_page_last               586
_journal_paper_doi               10.1107/S0108768109027177
_journal_volume                  65
_journal_year                    2009
_chemical_formula_sum            'Ba F4 Zn'
_chemical_formula_weight         278.7
_chemical_name_systematic        ' ?'
_space_group_IT_number           36
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_space_group_name_H-M   'C m c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.19057(2)
_cell_length_b                   14.512810(6)
_cell_length_c                   5.83568(3)
_cell_measurement_temperature    10
_cell_volume                     354.912(2)
_computing_cell_refinement       Jana2006
_computing_data_collection       'CRYSALIS CCD'
_computing_data_reduction        Jana2006
_computing_publication_material
'Jana2006 (Petricek, Dusek & Palatinus, 2006)'
_computing_structure_refinement
'Jana2006 (Petricek, Dusek & Palatinus, 2006)'
_diffrn_ambient_temperature      10
_diffrn_detector_area_resol_mean 8.3504
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Oxford Diffraction CCD'
_diffrn_measurement_method       \omega-scans
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0489
_diffrn_reflns_av_sigmaI/netI    0.0168
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -4
_diffrn_reflns_number            2878
_diffrn_reflns_reduction_process Jana2006
_diffrn_reflns_theta_full        36.66
_diffrn_reflns_theta_max         36.66
_diffrn_reflns_theta_min         2.81
_exptl_absorpt_coefficient_mu    17.713
_exptl_absorpt_correction_T_max  0.440
_exptl_absorpt_correction_T_min  0.182
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlis RED, Oxford Diffraction Ltd.,
Version 1.171.32.15 (release 10-01-2008 CrysAlis171 .NET)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.2144
_exptl_crystal_F_000             488
_exptl_crystal_size_max          0.1604
_exptl_crystal_size_mid          0.0958
_exptl_crystal_size_min          0.0500
_refine_diff_density_max         1.94
_refine_diff_density_min         -1.52
_refine_ls_abs_structure_details 'inversion twin'
_refine_ls_abs_structure_Flack   0.00(5)
_refine_ls_extinction_coef       19E1(2)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_ref   1.87
_refine_ls_number_constraints    1
_refine_ls_number_parameters     37
_refine_ls_number_reflns         538
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0224
_refine_ls_R_factor_gt           0.0219
_refine_ls_shift/su_max          0.0070
_refine_ls_shift/su_mean         0.0005
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0284
_refine_ls_wR_factor_ref         0.0285
_reflns_number_gt                524
_reflns_number_total             538
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            sn5085.cif
_cod_data_source_block           BaZnF410K
_cod_original_sg_symbol_Hall     'C -2x;-2yc;2zc'
_cod_original_formula_sum        'Ba1 F4 Zn1'
_cod_database_code               2104460
_cod_database_fobs_code          2104460